Hindawi Publishing Corporation e Scientiﬁc World Journal Volume 2014, Article ID 957904, 9 pages http://dx.doi.org/10.1155/2014/957904
Review Article Monitoring Corrosion of Steel Bars in Reinforced Concrete Structures Sanjeev Kumar Verma,1 Sudhir Singh Bhadauria,2 and Saleem Akhtar1 1
Civil Engineering Department, University Institute of Technology, Rajiv Gandhi Technical University, Airport Road, Bhopal, Madhya Pradesh 462036, India 2 Shri G.S. Institute of Technology and Science, Indore, Madhya Pradesh 452003, India Correspondence should be addressed to Sanjeev Kumar Verma; [email protected]
Received 11 August 2013; Accepted 20 October 2013; Published 16 January 2014 Academic Editors: H. Shih, ˙I. B. Topc¸u, and H.-H. Tsang Copyright © 2014 Sanjeev Kumar Verma et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited. Corrosion of steel bars embedded in reinforced concrete (RC) structures reduces the service life and durability of structures causing early failure of structure, which costs significantly for inspection and maintenance of deteriorating structures. Hence, monitoring of reinforcement corrosion is of significant importance for preventing premature failure of structures. This paper attempts to present the importance of monitoring reinforcement corrosion and describes the different methods for evaluating the corrosion state of RC structures, especially hal-cell potential (HCP) method. This paper also presents few techniques to protect concrete from corrosion.
1. Introduction Deterioration of concrete structures due to harsh environmental conditions leads to performance degradation of RC structures, and premature deterioration of structures before completing expected service life is major concern for engineers and researchers. Deterioration rate of structures depends on the exposure conditions and extent of maintenance. Corrosion, a result of chemical or electrochemical actions, is the most common mechanism responsible for deterioration of RC structures which is mainly governed by chloride ingress and carbonation depth of RC structures. Usually, there are two major factors which cause corrosion of rebars in concrete structures, carbonation and ingress of chloride ions. When chloride ions penetrate in concrete more than the threshold value or when carbonation depth exceeds concrete cover, then it initiates the corrosion of RC structures. If the corrosion is initiated in concrete structures, it progresses and reduces service life of the structures and rate of corrosion affects the remaining service life of RC structures. However, these severe environments can cause corrosion of reinforcement only if required amounts of oxygen and moisture are available at the rebar level in concrete structures . Corrosion of steel bars is the major cause of failure of concrete structures and about two tons of concrete is used
per capita of the world population every year. Therefore, it has been realized that durable structures will reduce the cement consumption. Corrosion can severely reduce the strength and life of structures and in humid conditions pollutants from atmosphere percolate through the concrete cover and cause corrosion of steel. After the initiation of corrosion in reinforcing steel, products of corrosion expand and occupy a volume of about 6–10 times greater than that of steel resulting in the formation of cracks and finally in the failure of structures as shown in Figures 1 and 2. Penetration of corrosion inducing agents such as chloride ions and carbon dioxide increased at the places of cracks, which further increases the corrosion . Corrosion in concrete structures can be prevented by using low permeable concrete which minimizes the penetration of corrosion inducing agent, and the high resistivity of concrete restricts the corrosion rate by reducing the flow of current from anode to cathode .
2. Half-Cell Potential Method Detection and evaluation of probability of corrosion in RC structures are essential. Proper corrosion monitoring of the concrete structures has been required for planning maintenance and replacement of the concrete structures. The most
The Scientific World Journal
Voltmeter Wet sponge
Reinforcing steel Concrete
Figure 3: Setup of half-cell potential measurement. Deterioration due to corrosion
Figure 1: Deterioration resulting from corrosion.
Figure 2: Cracks formation.
Figure 4: Half-cell potential contour.
appropriate repair strategy can be selected for a distressed concrete structure by determining the corrosion status of reinforcing bars . Repair of concrete structures without understanding the root cause of failure may be unsuccessful. If a cracked concrete patched without any treatment to the corroded steel, corrosion will likely continue and result in failure of patch work. Several methods for detecting corrosion activity discussed by authors in their previous paper  have been presented in Table 1. There are several methods available for detecting and evaluating the corrosion in reinforcement steel as presented in Table 1. However, half-cell potential has been recognized by many researchers as the main method to detect the corrosion activity in RC structures . In this method potential difference is measured between steel reinforcement and an external electrode with a voltmeter. The half-cell consists of a metal rod immersed in a solution of its own (Cu/CuSO4 or Ag/AgCl). The metal rod is connected with reinforcement steel by a voltmeter as shown in Figure 3. Some surface preparations including wetting to ensure good electrical connection are necessary. The main application of this method is in situ. External electrode and steel reinforcement are connected through a wet concrete cover as shown in Figure 3. Interpretation of results of half-cell potential measurement for reinforced concrete structures required high skills and experience, as this only provides information regarding the probability of corrosion instead of rate and nature of corrosion . Availability of oxygen, cover thickness, and concrete resistivity are few factors influencing the results of
half-cell potential test. This method evaluates the potential difference on the exposed surface of concrete structures. The potential can be measured at any point on the surface or average of several measurements taken from different points on the same surface may be considered for evaluating the probability of corrosion. More negative value of measured half-cell potential indicates more probability of corrosion, as indicated in Table 2 according to ASTM C876 for Cu/CuSO4 half-cell. This half-cell potential is also known as open circuit potential and is measured at several distinct points over a given area to be surveyed. Measured half-cell potential values can be used to plot a potential contour for the surface of reinforced concrete structure and this potential contour map as shown in Figure 4 can be used to evaluate the probability of corrosion at different points on the surface of the concrete structures. Portions of the structures likelihood of high corrosion activity can be obtained and identified by their high negative potentials.
3. Few Recently Conducted Corrosion Monitoring Activities Several techniques have been reported in previous literatures that can be used for monitoring and evaluating the corrosion of rebars in concrete structures for diagnosing the cause and effect of corrosion. Few such studies performed by different researchers have been presented in Table 3.
The Scientific World Journal
3 Table 1: Methods for evaluating corrosion in concrete structures .
Method Galvanostatic pulse method
Advantages Measures half-cell potential and electrical resistance simultaneously
Linear polarization resistance (LPR)
Rapid and requires only localized damage, more detailed information
Simple, portable, results in the form of equipotential contours
Time domain reflectometry (TDR)
More robust, easy, and locates corrosion and identifies extent of damage
By applying a sensor wire alongside of the reinforcement a transmission line is created. Physical defects of the reinforcement will change the electromagnetic properties of the line
Ultrasonic guided waves X-ray diffraction and atomic absorption
Identify location and magnitude of corrosion
Not very reliable
Based on propagation of ultrasonic waves
Simple and reliable
Intensity of X-ray beams reduces while passing through a material
Table 2: Presents criteria according to ASTM C876 for Cu/CuSO4 . S. no. 1 2 3
Half-cell potential (mV) >−200 −200 to −350